G1RTCT D. EXAMPLES F. GUTIÉRREZSOLANA S. CICERO J.A. ALVAREZ R. LACALLE W P 6: TRAINING & EDUCATION


 Denis Austin
 1 years ago
 Views:
Transcription
1 D. EXAMPLES 316
2 WORKED EXAMPLE I Infinite Plate under fatigue Introduction and Objectives Data Analysis 317
3 INTRODUCTION AND OBJECTIVES One structural component of big dimensions is subjected to variable loading conditions everyday: 200 MPa during 12 hours and 20 MPa the rest of the day. During the maximum loading conditions other variable stresses appear, with a variation of 30 MPa (because of vibrations with a frequency 50 Hz). Some NDT are performed, with equipment whose sensitivity is 0.2 mm and no cracks are detected. Considering the component as an infinite plate: a) Determine the crack length which is necessary to crack propagation because of vibrations b) Critical crack length for final failure c) Life time for the component d) Evolution of the crack length with time in order to determine inspection periods 318
4 DATA Material properties: K IC = 100 MPa m 1/2 ΔK th (or ΔK 0 ) = 3 MPa m 1/2 if R = P min /P max = 0.1 ΔK th = 1.5 MPa m 1/2 if R = P min /P max = 0.85 Paris Law: da dn = (ΔK) 2 da/dn in m/cycle when ΔK in MPa m 1/2 319
5 Working conditions are plotted in the next figure: σ ( M P a ) h 2 4 h t ( h ) 320
6 The component geometry can be simplified as: σ 2a 2W The equipment sensitivity is 0.2 mm and no crack has been detected. So, in the worst possible situation 2a = 0.2 mm. 321
7 State I: VIBRATIONS σ ( M P a ) h 2 4 h t ( h ) R = P max /P min = 0.8 ΔK th = 1.5 MPa m 1/2 ΔK = Δσ (π a) 1/2 = 30 (π ) 1/2 = 0.53 MPa m 1/2 < ΔK th Existing cracks don t propagate 322
8 State II: MAIN LOADING CONDITIONS σ ( M P a ) h 2 4 h t ( h ) As R = 0.10 ΔK th = 3.0 MPa m 1/2 ΔK = Δσ (π a) 1/2 = 180 (π ) 1/2 = 3.19 MPa m 1/2 > ΔK th Existing cracks could propagate 323
9 As existing cracks could propagate, it is necessary to determine the crack length for crack propagation because of vibrations: ΔK th = 1.5MPa m 1/2 = 30 π a v a v = 0.80 mm For shorter cracks propagation is only due to main loading variation (Δσ =180 MPa, f = 1/86400 Hz) The critical crack length determined at failure is: K a f I max = σ max = 68 mm π a c = 215 π a f = 100MPa m For crack length over 0.80 mm propagation is due to both main loading variation and vibrations (Δσ = 30 MPa, f = 5 Hz) 1/2 324
10 LIFE TIME: The time necessary to initiate the effects of vibrations to cause crack propagation is determined through the Paris law: 1 a f N = Ln = Ln = 2042 cycles C Y ( Δσ) π a 1 10 (180) π cycles is equivalent to 2042 days or 5.59 years Once this crack length is reached, propagation is due to vibrations (mainly): a 0 = 0.8 mm a f = 68 mm 1 a f 1 68 N = Ln = Ln C Y ( Δσ) π a (30) π cycles is equivalent to 0.73 days 2 = cycles The same day that cracks achive length to propagate due to vibration amplitude, the component fails. SO, LIFE TIME IS 5.59 YEARS. 325
11 The evolution of semicrack length with time is (question d)): a ( m m ) 6 8 It is reasonable to define periodical inspections to check if really cracks propagate over the detectable value of 0.2 mm in total length (i.e. every two years) inspection in 2 years. cracks detected? No 0, 8 0, 1 5,59 ye a r s Yes Evaluate remanent life and take decisions 326
12 WORKED EXAMPLE II Fatigue test Introduction and data Objectives Analysis 327
13 INTRODUCTION AND DATA A fatigue test on a seven wire strand was performed. The maximum applied stress is 0.8 σ u and the amplitude is 390 MPa. The strand is one meter long and the diameter of the wires is 5 mm. The test finished with three broken wires, the central one and two external (which were together), after fatigue cycles (f = 8 Hz). The SEM observation of the failure surfaces gave the following information about crack lengths:  Central wire: 0.25 mm (depth) elliptical crack from non propagated initial defect.  External wire A: 1.32 mm from a non differentiated initial defect.  External wire B: 1.20 mm proceeding from a 0.30 mm in depth initial defect. From a previous tension test, the mechanical behaviour of the strand was obtained: E = 195 GPa Failure Load = kn Strain for Failure Load = 4.7 % (gauge base 500 mm) 328
14 OBJECTIVES From the testing results and the behaviour of the material, determine: a) The failure sequence of the wires as well as their form of failure and the fracture toughness of the material. b) Fatigue behaviour of the material considering a Paris exponent of 2.4 and the depth of the initial defect of wire A. a Consider for the wire geometry that K I = 2.12 σ a
15 The area of each wire is: A w = π r 2 = π = mm 2 Therefore, the area of the strand is A = 7 A w = = mm 2 The failure load is kn, so the failure stress can be calculated: σ f = / =1864 MPa The maximum and minimum stresses are: σ max = 0.8 σ f = = MPa σ min = 0.8 σ f 390 = = MPa 330
16 Under these conditions, the first failure occurs in the external wire A because it has the bigger propagated defect. After that, the external wire B breaks and finally, the central one. The external wire A breaks because of a fracture failure as a consequence of a fatigue process. Then: K I = 2.12 σ a c 0.5 = ( ) 0.5 = MPa m 1/2 K IC = MPa m ½ 331
17 The external wire B also fails because of fracture, but with a smaller defect because the decrease of the section once the external wire A is broken. The new supported σ max is: σ max = 7/ = MPa This stress is smaller than the failure strength of the strand (1864 MPa). Therefore, failure happens as a consequence of sudden fracture or plastic collapse. This later as the applied stress ( MPa) is close to yield stress (even non considering a possible strain hardening effect, then σ ymax = σ u = 1864 MPa) 332
18 We can calculate the stress intensity factor: K I = 2.12 σ a c 0.5 = (0.0012) 0.5 K I = MPa m ½ This value is bigger than K IC and it justifies the sudden failure of the external wire B. Now, there are only five wires in the section of the strand, so: σ max = 6/ = MPa This stress is bigger than the failure stress of the cord (1864 MPa). Therefore, it is possible to affirm that the latest is the maximum stress in the strand, and the central wire fails because of tension. In effect, the necessary stress for fracture to occur would be: = 2.12 σ σ = 3428 MPa Such a value is not reached at any time. 333
19 Let s now determine the fatigue properties of the material. We know that the central wire had a defect of 0.25 mm which did not produce crack propagation under Δσ = 390 MPa. So: ΔK th > 2.12 Δσ a 0.5 = = MPa m 1/2 We also know that an initial defect of 0.3 mm propagates in the external wire B and that the unknown initial defect of wire A should be higher than 0.3 because it reached a bigger final crack. So: ΔK th < 2.12 Δσ a 0.5 = = MPa m 1/2 From both expressions the threshold SIF is limited from the following values: < ΔK th < MPa m 1/2 334
20 The Paris law is: da dn 2.4 = C ( ΔK) = C (2.12 Δσ a ) 2.4 where C has to be defined We know: Δσ = 390 MPa So: da dn = C ( 2.4 ΔK ) = C ( a ) a i a f = da 2. C ( ) 4 dn 1.2 a = a = 0.3 mm C N a i f = 1.2 mm N = cycles conditions at wire B 335
21 C = = Therefore, the Paris law is: da dn = ( ΔK) 2.4 To calculate the initial defect in the external wire A, we will integrate the Paris law: 12 C = a 0.2 i a f = C N a f = 1.32 mm N = cycles a i = C N = a i = mm 336
C. PROCEDURE APPLICATION (FITNET)
C. PROCEDURE APPLICATION () 495 INTRODUCTION ASSESSMENT OF SCC ASSESSMENT OF CORROSION FATIGUE STRESS CORROSION AND CORROSION FATIGUE ANALYSIS ASSESSMENT OF LOCAL THINNED AREAS 496 INTRODUCTION INTRODUCTION
More informationFatigue Testing. Objectives
Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students
More informationPrinciples of Fracture Mechanics
81 CHAPTER 8 FAILURE PROBLEM SOLUTIONS Principles of Fracture Mechanics 8.1 This problem asks that we compute the magnitude of the maximum stress that exists at the tip of an internal crack. Equation
More informationFatigue crack propagation
1 (20) Repetition Ð Crack initiation and growth Small cracks Shear driven Interact with microstructure Mostly analyzed by continuum mechanics approaches Large cracks Tension driven Fairly insensitive to
More informationB. INTRODUCTION TO ASSESSMENT PROCEDURES FOR CRACKED COMPONENTS
B. INTRODUCTION TO ASSESSMENT PROCEDURES FOR CRACKED COMPONENTS 40 INTRODUCTION HOW ARE INTEGRITY, SECURITY OR CRITICAL CONDITIONS ANALYSED IN A CRACKED STRUCTURE? FRACTURE MECHANICS Critical conditions
More information9. TIME DEPENDENT BEHAVIOUR: CYCLIC FATIGUE
9. TIME DEPENDENT BEHAVIOUR: CYCLIC FATIGUE A machine part or structure will, if improperly designed and subjected to a repeated reversal or removal of an applied load, fail at a stress much lower than
More informationσ m using Equation 8.1 given that σ
8. Etimate the theoretical fracture trength of a brittle material if it i known that fracture occur by the propagation of an elliptically haped urface crack of length 0.8 mm and having a tip radiu of curvature
More informationG1RTCT200105071 A. BASIC CONCEPTS F. GUTIÉRREZSOLANA S. CICERO J.A. ALVAREZ R. LACALLE W P 6: TRAINING & EDUCATION
A. BASIC CONCEPTS 472 PROCESSES LOADING RATE Static or QuasiSstatic Dynamic MATERIAL ENVIRONMENT Liquid or Gaseous Environments AGGRESSIVE ENVIRONMENT MECHANIC LOADS Stress corrosion cracking (SCC) Corrosion
More informationME111 Lecture 16 1. ME111 Instructor: Peter Pinsky Class #16 November 1, 2000
Toda s Topics ME111 Instructor: Peter Pinsk Class #16 November 1, 2000 Introduction to linear elastic fracture mechanics (LEFM). Problem 3 A centercracked plate of AII 1144 steel ( C = 115MPa m ) has
More informationDamage due to fatigue occurs when loading is markedly varying in time. R decreases with time S T. MSÚ F max
5. Fatigue of steel structures Fatigue loading, Wöhler s approach and fracture mechanics, fatigue strength, influence of notches, damage accumulation, Eurocode approach. Damage due to fatigue occurs when
More informationMechanical Metallurgy
Mechanical Metallurgy Lecturer Assessment Dr. Assignment 20 (homework, quiz, attendance) Midterm exam 40 Final exam 40 Total 100 Mechanical Metallurgy Subject of interests Part I Mechanical fundamentals
More informationCH 6: Fatigue Failure Resulting from Variable Loading
CH 6: Fatigue Failure Resulting from Variable Loading Some machine elements are subjected to static loads and for such elements static failure theories are used to predict failure (yielding or fracture).
More informationANALYSIS OF THE FATIGUE STRENGTH UNDER TWO LOAD LEVELS OF A STAINLESS STEEL BASED ON ENERGY DISSIPATION
EPJ Web of Conferences 6, 6 38009 (00) DOI:0.05/epjconf/000638009 Owned by the authors, published by EDP Sciences, 00 ANALYSIS OF THE FATIGUE STRENGTH UNDER TWO LOAD LEVELS OF A STAINLESS STEEL BASED ON
More informationNOTCHES AND THEIR EFFECTS. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1
NOTCHES AND THEIR EFFECTS Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1 CHAPTER OUTLINE Background Stress/Strain Concentrations SN Approach for Notched Members
More informationObjective To conduct Charpy Vnotch impact test and determine the ductilebrittle transition temperature of steels.
IMPACT TESTING Objective To conduct Charpy Vnotch impact test and determine the ductilebrittle transition temperature of steels. Equipment Coolants Standard Charpy VNotched Test specimens Impact tester
More informationSTRAINLIFE (e N) APPROACH
CYCLIC DEFORMATION & STRAINLIFE (e N) APPROACH MONOTONIC TENSION TEST AND STRESSSTRAIN BEHAVIOR STRAINCONTROLLED TEST METHODS CYCLIC DEFORMATION AND STRESSSTRAIN BEHAVIOR STRAINBASED APPROACH TO
More informationdifferent levels, also called repeated, alternating, or fluctuating stresses.
Fatigue and Dynamic Loading 1 Fti Fatigue fil failure: 2 Static ti conditions : loads are applied gradually, to give sufficient i time for the strain to fully develop. Variable conditions : stresses vary
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationAccelerated Corrosion Fatigue Studies on SA 333 Gr.6 Carbon Steel
Accelerated Corrosion Fatigue Studies on SA 333 Gr.6 Carbon Steel P. S. Aarthi 1, G. Raghava 2, S. Vishnuvardhan 3, M. Surendar 4 P.G. Student, Department of Civil Engineering, Easwari Engineering College,
More informationIMPELLER FATIGUE ASSESSMENT USING AN SN APPROACH
ENGINEERING PAPER 524408 IMPELLER FATIGUE ASSESSMENT USING AN SN APPROACH Samuel Orr Engineering Analysis Manager Howden Technology AMCA International Engineering Conference Las Vegas, NV, USA 2 4 March
More information( ) = ( ) = {,,, } β ( ), < 1 ( ) + ( ) = ( ) + ( )
{ } ( ) = ( ) = {,,, } ( ) β ( ), < 1 ( ) + ( ) = ( ) + ( ) max, ( ) [ ( )] + ( ) [ ( )], [ ( )] [ ( )] = =, ( ) = ( ) = 0 ( ) = ( ) ( ) ( ) =, ( ), ( ) =, ( ), ( ). ln ( ) = ln ( ). + 1 ( ) = ( ) Ω[ (
More informationInvestigation of Stress Intensity Factor of Axial Compressor Blade of Helicopter
Investigation of Stress Intensity Factor of Axial Compressor Blade of Helicopter Neelesh V K Mr. Manjunath M V Mr. Devaraj Dept. of Mechanical Engineering Asst prof, Dept. of Mechanical Engineering Asst
More informationREHABILITATION OF THE FIGUEIRA DA FOZ BRIDGE
REHABILITATION OF THE FIGUEIRA DA FOZ BRIDGE A.Rito Proponte, Lda, Lisbon, Portugal J. Appleton A2P Consult, Lda, Lisbon, Portugal ABSTRACT: The Figueira da Foz Bridge includes a 405 m long cable stayed
More informationDescription of mechanical properties
ArcelorMittal Europe Flat Products Description of mechanical properties Introduction Mechanical properties are governed by the basic concepts of elasticity, plasticity and toughness. Elasticity is the
More informationMultiaxial Fatigue. Professor Darrell Socie. 20082014 Darrell Socie, All Rights Reserved
Multiaxial Fatigue Professor Darrell Socie 20082014 Darrell Socie, All Rights Reserved Outline Stresses around holes Crack Nucleation Crack Growth MultiaxialFatigue 20082014 Darrell Socie, All Rights
More informationFatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY)
Fatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY) Ali Fatemi, Jonathan Williams and Farzin Montazersadgh Professor and Graduate
More informationMaster of Simulation Techniques. Lecture No.5. Blanking. Blanking. Fine
Master of Simulation Techniques Lecture No.5 Fine Blanking Prof. Dr.Ing. F. Klocke Structure of the lecture Blanking Sheared surface and force Wear Blanking processes and blanking tools Errors on sheared
More informationLecture 14. Chapter 81
Lecture 14 Fatigue & Creep in Engineering Materials (Chapter 8) Chapter 81 Fatigue Fatigue = failure under applied cyclic stress. specimen compression on top bearing bearing motor counter flex coupling
More informationTensile Testing of Steel
C 265 Lab No. 2: Tensile Testing of Steel See web for typical report format including: TITL PAG, ABSTRACT, TABL OF CONTNTS, LIST OF TABL, LIST OF FIGURS 1.0  INTRODUCTION See General Lab Report Format
More informationValidation of Cable Bolt Support Design in Weak Rock Using SMART Instruments and Phase 2
Validation of Cable Bolt Support Design in Weak Rock Using SMART Instruments and Phase 2 W.F. Bawden, Chair Lassonde Mineral Engineering Program, U. of Toronto, Canada J.D. Tod, Senior Engineer, Mine Design
More informationSolved with COMSOL Multiphysics 4.3
Vibrating String Introduction In the following example you compute the natural frequencies of a pretensioned string using the 2D Truss interface. This is an example of stress stiffening ; in fact the
More informationLOADCARRYING CAPACITY OF AXIALLY LOADED RODS GLUEDIN PERPENDICULAR TO THE GRAIN
LOADCARRYING CAPACITY OF AXIALLY LOADED RODS GLUEDIN PERPENDICULAR TO TE GRAIN Prof. Dr.Ing..J. Blaß, Dipl.Ing. B. Laskewitz Universität Karlsruhe (T), Germany Abstract Gluedin rods have been used
More informationStructural Integrity Analysis
Structural Integrity Analysis 1. STRESS CONCENTRATION Igor Kokcharov 1.1 STRESSES AND CONCENTRATORS 1.1.1 Stress An applied external force F causes inner forces in the carrying structure. Inner forces
More informationPROPERTIES OF MATERIALS
1 PROPERTIES OF MATERIALS 1.1 PROPERTIES OF MATERIALS Different materials possess different properties in varying degree and therefore behave in different ways under given conditions. These properties
More informationFATIGUE ANALYSES OF AERONAUTICAL STRUCTURAL DETAILS OF DIFFERENT COMPLEXITY
FATIGUE ANALYSES OF AERONAUTICAL STRUCTURAL DETAILS OF DIFFERENT COMPLEXITY Paulo M S T de Castro, Paulo F P de Matos, Pedro M G P Moreira, Lucas F M da Silva IDMEC and Faculdade de Engenharia, Universidade
More informationThe Mechanical Properties of Glass
The Mechanical Properties of Glass Theoretical strength, practical strength, fatigue, flaws, toughness, chemical processes Glass Engineering 150:312 Professor Richard Lehman Department of Ceramics and
More informationDesign strength of optical glass
Design strength of optical glass Keith B. Doyle Sigmadyne, Inc. Rochester, NY Mark A. Kahan Optical Research Associates Westborough, MA ABSTRACT Brittle materials such as glass do not possess a single
More information2. FRACTURE MECHANICS
2. FRACTURE MECHANICS Igor Kokcharov 2.1 DEFECTS Structural materials have inner defects such as cracks, which are extreme stress concentrators. There are technological defects shown in diagrams A and
More informationDentistry Fatigue test for endosseous dental implants. Report No.: 1 ASTRA System Ti Design
Dentistry Fatigue test for endosseous dental implants Report No.: 1 ASTRA System Ti Design Client: NT  Trading Time of execution: Mai 2011 Subject of work:   S  24285 Abutment Ti DesignTM  RESULTS
More informationALLOY 7475 PLATE AND SHEET HIGHEST TOUGHNESS/STRENGTH
ALCOA MILL PRODUCTS ALLOY 7475 PLATE AND SHEET HIGHEST TOUGHNESS/STRENGTH ALLOY 7475 DESCRIPTION Alloy 7475 is a controlled toughness alloy developed by Alcoa for sheet and plate applications that require
More informationPOLITECNICO DI TORINO. Engineering Faculty Master s Degree in Aerospace Engineering. Final Thesis
POLITECNICO DI TORINO Engineering Faculty Master s Degree in Aerospace Engineering Final Thesis DETECTION AND ANALYSIS OF BARELY VISIBLE IMPACT DAMAGE AND ITS PROGRESSION ON A COMPOSITE OVERWRAPPED PRESSURE
More informationMETU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING
METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING Met E 206 MATERIALS LABORATORY EXPERIMENT 1 Prof. Dr. Rıza GÜRBÜZ Res. Assist. Gül ÇEVİK (Room: B306) INTRODUCTION TENSION TEST Mechanical testing
More informationMODELING THE EFFECT OF TEMPERATURE AND FREQUENCY ON BITUMENCOATED HELICAL CABLE ELEMENTS
MODELING THE EFFECT OF TEMPERATURE AND FREQUENCY ON BITUMENCOATED HELICAL CABLE ELEMENTS Bjørn Konradsen 1 Technological Analyses Centre, Hybrid Underwater Cables, Nexans Norway Steinar V. Ouren Material
More informationNumerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope
Numerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope Rakesh Sidharthan 1 Gnanavel B K 2 Assistant professor Mechanical, Department Professor, Mechanical Department, Gojan engineering college,
More informationTensile fracture analysis of blunt notched PMMA specimens by means of the Strain Energy Density
Engineering Solid Mechanics 3 (2015) 3542 Contents lists available at GrowingScience Engineering Solid Mechanics homepage: www.growingscience.com/esm Tensile fracture analysis of blunt notched PMMA specimens
More informationProperties of Materials
CHAPTER 1 Properties of Materials INTRODUCTION Materials are the driving force behind the technological revolutions and are the key ingredients for manufacturing. Materials are everywhere around us, and
More informationFEM analysis of the forming process of automotive suspension springs
FEM analysis of the forming process of automotive suspension springs Berti G. and Monti M. University of Padua, DTG, Stradella San Nicola 3, I36100 Vicenza (Italy) guido.berti@unipd.it, manuel.monti@unipd.it.
More informationUltrasonic Technique and Device for Residual Stress Measurement
Ultrasonic Technique and Device for Residual Stress Measurement Y. Kudryavtsev, J. Kleiman Integrity Testing Laboratory Inc. 80 Esna Park Drive, Units 79, Markham, Ontario, L3R 2R7 Canada ykudryavtsev@itlinc.com
More informationFRETTING FATIGUE UNDER VARYING LOADING BELOW THE FRETTING FATIGUE LIMIT
FRETTING FATIGUE UNDER VARYING LOADING BELOW THE FRETTING FATIGUE LIMIT Yoshiyuki KONDO 1, Chu SAKAE 1, Masanobu KUBOTA 1 and Hiroki KITAHARA 2 1 Kyushu University, Faculty of Engineering, 6101, Hakozaki,
More informationMeasuring the Condition of Prestressed Concrete Cylinder Pipe
Measuring the Condition of Prestressed Concrete Cylinder Pipe John Marshall, P.E.I, I J.W. Marshall and Associates, and Paul S. Fisk, President NDT Corporation Introduction Prestressed Concrete Cylinder
More informationNumerical modelling of shear connection between concrete slab and sheeting deck
7th fib International PhD Symposium in Civil Engineering 2008 September 1013, Universität Stuttgart, Germany Numerical modelling of shear connection between concrete slab and sheeting deck Noémi Seres
More informationUniaxial Tension and Compression Testing of Materials. Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng
Uniaxial Tension and Compression Testing of Materials Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng 3.032 Lab Report September 25, 2013 I. Introduction Understanding material mechanics
More informationPunching shear behavior of steelconcrete composite decks with different shear connectors
Punching shear behavior of steelconcrete composite decks with different shear connectors *XiaoQing Xu 1) and YuQing Liu 2) 1), 2) Department of Bridge Engineering, Tongji University, Shanghai 200092,
More informationSDNS108 Dynamic response of a reinforced concrete slab leaned on 4 with dimensions subjected to a concentrated loading
Titre : SDNS108  Réponse dynamique d'une dalle en béton a[...] Date : 31/05/2012 Page : 1/9 SDNS108 Dynamic response of a reinforced concrete slab leaned on 4 with dimensions subjected to a concentrated
More informationOptimum proportions for the design of suspension bridge
Journal of Civil Engineering (IEB), 34 (1) (26) 114 Optimum proportions for the design of suspension bridge Tanvir Manzur and Alamgir Habib Department of Civil Engineering Bangladesh University of Engineering
More informationYield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials. τ xy 2σ y. σ x 3. τ yz 2σ z 3. ) 2 + ( σ 3. σ 3
Yield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials Brittle materials are materials that display Hookean behavior (linear relationship between stress and strain) and which
More informationTENSILE TESTING PRACTICAL
TENSILE TESTING PRACTICAL MTK 2B Science Of Materials Ts epo Mputsoe 215024596 Summary Material have different properties all varying form mechanical to chemical properties. Taking special interest in
More informationWELD  STATIC AND FATIGUE STRENGTH III
32 WELD  STATIC AND FATIGUE STRENGTH III 1.0 INTRODUCTION A component or a structure, which can withstand a single application of load, may fracture if the same load is applied a large number of times.
More informationFlexural Strength of Concrete (The Modulus of Rupture Test)
Revised 09063, WKS Datasheet No. 7.6a & 7.6b MOHAWK COLLEGE OF APPLIED ARTS AND TECHNOLOGY BUILDING AND CONSTRUCTION SCIENCES DEPARTMENT Flexural Strength of Concrete (The Modulus of Rupture Test) INTRODUCTION
More information7.2.4 Seismic velocity, attenuation and rock properties
7.2.4 Seismic velocity, attenuation and rock properties Rock properties that affect seismic velocity Porosity Lithification Pressure Fluid saturation Velocity in unconsolidated near surface soils (the
More informationWires and Strands for Prestressed Concrete
Wires and Strands for Prestressed Concrete Raw Materials Manufacturing Process Wires 1 Wires and Strands for Prestressed Concrete 1.1 Wires EMCOCABLES manufactures a wide variety of wires with a high
More informationBending, Forming and Flexing Printed Circuits
Bending, Forming and Flexing Printed Circuits John Coonrod Rogers Corporation Introduction: In the printed circuit board industry there are generally two main types of circuit boards; there are rigid printed
More informationHardened Concrete. Lecture No. 14
Hardened Concrete Lecture No. 14 Strength of Concrete Strength of concrete is commonly considered its most valuable property, although in many practical cases, other characteristics, such as durability
More informationExperiment: Fatigue Testing
Experiment: Fatigue Testing Objectives  To demonstrate the use of the Instron servohydraulic testing machine for testing specimens subjected to cyclic (fatigue) loadings.  To analytically approximate
More informationTechnical Report Example (1) Chartered (CEng) Membership
Technical Report Example (1) Chartered (CEng) Membership A TECHNICAL REPORT IN SUPPORT OF APPLICATION FOR CHARTERED MEMBERSHIP OF IGEM DESIGN OF 600 (103 BAR) 820MM SELF SEALING REPAIR CLAMP AND VERIFICATION
More informationFracture Mechanics Assessment of highly loaded cast iron components for low temperature. Dr. Peter Langenberg
Fracture Mechanics Assessment of highly loaded cast iron components for low temperature Dr. Peter Langenberg IWT (Ingenieurbüro für Werkstofftechnik) Aachen Cast Tec 2012 Krefeld, November2012 1,00E+00
More informationTENSIONMETER ** code 183_LNRSTW **
Electronic tension meter for applications in textile and wire industry. 9 Tension ranges from 0.1200 cn to 550 dan. Versatile instruments usable for applications in textile industry: e. g. 50 up to max.
More informationObjectives. Experimentally determine the yield strength, tensile strength, and modules of elasticity and ductility of given materials.
Lab 3 Tension Test Objectives Concepts Background Experimental Procedure Report Requirements Discussion Objectives Experimentally determine the yield strength, tensile strength, and modules of elasticity
More informationFATIGUE LIFE OF BOLT SUBJECTED TO FATIGUE LOADING CONDITIONS
20 FATIGUE LIFE OF BOLT SUBJECTED TO FATIGUE LOADING CONDITIONS ABSTRACT K. Din and M. T. H. Ghazali Faculty of Civil Engineering, Universiti Teknologi MARA, Shah Alam, Malaysia Email: kdfila@hotmail.com
More informationFatigue Resistance of High Strength Bolts with Large Diameters
1 Fatigue Resistance of High Strength Bolts with Large Diameters Prof. Peter Schaumann; Dipl.Ing. Frithjof Marten Leibniz Universitaet Hannover Institute for Steel Construction Hannover, Germany schaumann@stahl.unihannover.de;
More informationFATIGUE CONSIDERATION IN DESIGN
FATIGUE CONSIDERATION IN DESIGN OBJECTIVES AND SCOPE In this module we will be discussing on design aspects related to fatigue failure, an important mode of failure in engineering components. Fatigue failure
More informationThe Bending Strength of Pasta
The Bending Strength of Pasta 1.105 Lab #1 Louis L. Bucciarelli 9 September, 2003 Lab Partners: [Name1] [Name2] Data File: Tgroup3.txt On the cover page, include your name, the names of your lab partners,
More informationSheet metal operations  Bending and related processes
Sheet metal operations  Bending and related processes R. Chandramouli Associate DeanResearch SASTRA University, Thanjavur613 401 Table of Contents 1.QuizKey... Error! Bookmark not defined. 1.Bending
More informationTENSILE BEHAVIOUR OF OPEN CELL CERAMIC FOAMS
Original papers TENSILE BEHAVIOUR OF OPEN CELL CERAMIC FOAMS LUKÁŠ ŘEHOŘEK*, **, IVO DLOUHÝ*,**, ZDENĚK CHLUP* *Institute of Physics of Materials ASCR, Žižkova 22, 616 62 Brno, Czech Republic **Institute
More informationFailure Analysis of a Cast A380 Aluminum Alloy Casting Using a Microstructurally Based Fatigue Model
Failure Analysis of a Cast A380 Aluminum Alloy Casting Using a Microstructurally Based Fatigue Model C.L. Burton, M.K. Jones, D.L. Oglesby A.L. Oppedal, M.Q. Chandler, M.F. Horstemeyer Center for Advanced
More informationOperating Temperature Range: 30 to +85ç (Note 1) Operating Humidity Range: 40 to 80%
All non products have been discontinued, or will be discontinued soon. Please check the products status on the Hirose website search at www.hiroseconnectors.com, or contact your Hirose sales representative.
More informationTopology Optimization of Engine Mount Brackets Dr. Dirk Sprengel Ford Werke GmbH
Topology Optimization of Engine Mount Brackets Dr. Dirk Sprengel Ford Werke GmbH Dr. D. Sprengel 6/2007 Topology Optimization of EMS Bracket 1 ( 21 ) EMS Bracket Funktion EMS: Engine Mount System Link
More informationHigh tensile steel wire and strand for the prestressing of concrete Specification
High tensile steel wire and strand for the prestressing
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationBolting Galvanized Steel
Bolting Galvanized Steel This chapter gives information on the characteristics, advantages and economics of bolted galvanized structures and zinc coated fasteners, and offers comment on bolting procedures
More informationAnalysis of Slotted Counter Sunk (35NCD16 Steel) Aerospace Fasteners
Analysis of Slotted Counter Sunk (35NCD16 Steel) Aerospace Fasteners A R Abelin Roy Deptt. of ME, Govt. Engineering College, Thrissur, India Christopher Solomon S MMD VSSC, ISRO Thiruvananthapuram, India
More informationCRITERIA FOR PRELOADED BOLTS
National Aeronautics and Space Administration Lyndon B. Johnson Space Center Houston, Texas 77058 REVISION A JULY 6, 1998 REPLACES BASELINE SPACE SHUTTLE CRITERIA FOR PRELOADED BOLTS CONTENTS 1.0 INTRODUCTION..............................................
More informationFATIGUE TESTS AND STRESSLIFE (SN) APPROACH
FATIGUE TESTS AND STRESSLIFE (SN) APPROACH FATIGUE TESTING LOADING TEST MACHINES SPECIMENS STANDARDS STRESSLIFE APPEROACH SN CURVES MEAN STRESS EFFECTS ON SN BEHAVIOR FACTORS INFLUENCING SN BEHAVIOR
More informationEDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME 2 ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS
ENGINEERING COMPONENTS EDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS Structural members: struts and ties; direct stress and strain,
More informationANALYSIS OF A LAP JOINT FRICTION CONNECTION USING HIGH STRENGTH BOLTS
Nordic Steel Construction Conference 212 Hotel Bristol, Oslo, Norway 57 September 212 ANALYSIS OF A LAP JOINT FRICTION CONNECTION USING HIGH STRENGTH BOLTS Marouene Limam a, Christine Heistermann a and
More informationIntroduction to Solid Modeling Using SolidWorks 2012 SolidWorks Simulation Tutorial Page 1
Introduction to Solid Modeling Using SolidWorks 2012 SolidWorks Simulation Tutorial Page 1 In this tutorial, we will use the SolidWorks Simulation finite element analysis (FEA) program to analyze the response
More informationModelling of fatigue crack growth in Inconel 718 under hold time conditions  application to a flight spectrum
Modelling of fatigue crack growth in Inconel 718 under hold time conditions  application to a flight spectrum Erik Lundström, Kjell Simonsson, Tomas Månsson and David Gustafsson Linköping University Post
More informationThere are as many reasons to test metals as there are metals:
Testing Their Mettle Metals testing procedures ensure quality in raw materials and finished products BY BILL O NEIL, ADRIAN RIDDICK, FRANK LIO, PAUL KING, CHRIS WILSON, AND PATTY HARTZELL There are as
More informationChapter 17: Springs. Fundamentals of Machine Elements, 3 rd ed. Schmid, Hamrock and Jacobson. 2014 CRC Press
Chapter 17: Springs It must be confessed that the inventors of the mechanical arts have been much more useful to men than the inventors of syllogisms. Voltaire A collection of helical compression springs.
More informationMechanical Properties
Mechanical Properties Hardness Hardness can be defined as resistance to deformation or indentation or resistance to scratch. Hardness Indentation Scratch Rebound Indentation hardness is of particular interest
More informationFatigue. 3. Final fracture (rough zone) 1. Fatigue origin. 2. Beach marks (velvety zone)
Fatigue Term fatigue introduced by Poncelet (France) 1839 progressive fracture is more descriptive 1. Minute crack at critical area of high local stress (geometric stress raiser, flaws, preexisting cracks)
More informationIntegrity assessment of grouted posttensioning cables and reinforced concrete of a nuclear containment building
EPJ Web of Conferences 12, 02002 (2011) DOI: 10.1051/epjconf/20111202002 C Owned by the authors, published by EDP Sciences, 2011 Integrity assessment of grouted posttensioning cables and reinforced concrete
More informationEvaluation of Soft Soldering on Aluminium Nitride (AlN) ESTEC Contract No. 19220/05/NL/PA. CTB Hybrids WG ESTEC22nd May 2007
Evaluation of Soft Soldering on Aluminium Nitride (AlN) ESTEC Contract No. 19220/05/NL/PA CTB Hybrids WG ESTEC22nd May 2007 Evaluation of Soft Soldering on AlN Schedule Project presentation Feasibility
More informationElectroless Nickel / Immersion Gold Process Technology for Improved Ductility of Flex and RigidFlex Applications
M44.44kkgrowth Electroless Nickel / Immersion Gold Process Technology for Improved Ductility of Flex and RigidFlex Applications By: Kuldip Johal and Hugh Roberts  Atotech USA Inc. Sven Lamprecht and
More informationEDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES AND APPLICATIONS NQF LEVEL 3 OUTCOME 1  LOADING SYSTEMS TUTORIAL 3 LOADED COMPONENTS
EDEXCEL NATIONAL CERTIICATE/DIPLOMA MECHANICAL PRINCIPLES AND APPLICATIONS NQ LEVEL 3 OUTCOME 1  LOADING SYSTEMS TUTORIAL 3 LOADED COMPONENTS 1. Be able to determine the effects of loading in static engineering
More informationDAMPED VIBRATION ANALYSIS OF COMPOSITE SIMPLY SUPPORTED BEAM
International Journal of Mechanical Engineering and Technology (IJMET) Volume 6, Issue 11, Nov 15, pp. 106113, Article ID: IJMET_06_11_013 Available online at http://www.iaeme.com/ijmet/issues.asp?jtype=ijmet&vtype=6&itype=11
More informationThe EJOT. Fastener. Predictable performance improvement for thermoplastics. EJOT The Quality Connection
The EJOT Fastener Predictable performance improvement for thermoplastics EJOT The Quality Connection Benefits of the EJOT DELTA PT The product Minimal radial tension due to optimized flank angle High clamp
More informationShort and Large Crack, MixedMode FatigueCrack Growth Thresholds in Ti6Al4V 1
Short and Large Crack, MixedMode FatigueCrack Growth Thresholds in Ti6Al4V 1 Mr. R. K. Nalla, Dr. J. P. Campbell and Professor R. O. Ritchie 2 Department of Materials Science and Engineering University
More informationMECHANICS OF SOLIDS  BEAMS TUTORIAL TUTORIAL 4  COMPLEMENTARY SHEAR STRESS
MECHANICS OF SOLIDS  BEAMS TUTORIAL TUTORIAL 4  COMPLEMENTARY SHEAR STRESS This the fourth and final tutorial on bending of beams. You should judge our progress b completing the self assessment exercises.
More informationEVALUATION OF SEISMIC RESPONSE  FACULTY OF LAND RECLAMATION AND ENVIRONMENTAL ENGINEERING BUCHAREST
EVALUATION OF SEISMIC RESPONSE  FACULTY OF LAND RECLAMATION AND ENVIRONMENTAL ENGINEERING BUCHAREST Abstract Camelia SLAVE University of Agronomic Sciences and Veterinary Medicine of Bucharest, 59 Marasti
More information